Lanthanide separation using size-selective crystallization of Ln-MOFs
Luo, Feng; Gao, Heng Ya; Peng, Wenli; Meng, PanPan; Feng, Xuefeng; Li, Jianqiang; Wu, HuiQiong; Yan, Chang Sheng; Xiaong, Yang Yang; Chem. Commun.  (2017) –; doi:10.1039/C7CC01898C

data_7120034
_publ_section_title
;
 Lanthanide separation using size-selective crystallization of Ln-MOFs
;
_journal_name_full               'Chem. Commun.'
_journal_paper_doi               10.1039/C7CC01898C
_journal_year                    2017
_chemical_formula_moiety         'C96 H100 Cu6 P6 Sn2 Te6, 2(C7 H8)'
_chemical_formula_sum            'C110 H116 Cu6 P6 Sn2 Te6'
_chemical_formula_weight         3008.06
_chemical_name_systematic
; 
 ? 
;
_chemical_properties_physical
', Air-sensitive,Moisture-sensitive,Oxygen-sensitive'
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014
_audit_update_record
;
2017-03-10 deposited with the CCDC.
2017-04-27 downloaded from the CCDC.
;
_cell_angle_alpha                73.848(4)
_cell_angle_beta                 69.207(3)
_cell_angle_gamma                70.959(3)
_cell_formula_units_Z            1
_cell_length_a                   14.4576(6)
_cell_length_b                   14.5360(6)
_cell_length_c                   14.6347(8)
_cell_measurement_reflns_used    32247
_cell_measurement_temperature    180(2)
_cell_measurement_theta_max      27.33
_cell_measurement_theta_min      2.33
_cell_volume                     2671.7(2)
_computing_cell_refinement       'STOE X-AREA'
_computing_data_collection       'STOE X-AREA'
_computing_data_reduction        'STOE X-RED'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2014 (Sheldrick, 2014)'
_diffrn_ambient_temperature      180(2)
_diffrn_detector_area_resol_mean 6.67
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.982
_diffrn_measurement_device_type  'STOE IPDS 2T'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0340
_diffrn_reflns_av_unetI/netI     0.0324
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.982
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -18
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            24851
_diffrn_reflns_point_group_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.982
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.802
_diffrn_reflns_theta_min         2.427
_diffrn_source
'sealed X-ray tube, 12 x 0.4 mm long-fine focus'
_exptl_absorpt_coefficient_mu    3.371
_exptl_absorpt_correction_T_max  0.7055
_exptl_absorpt_correction_T_min  0.4429
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   XRED32
_exptl_crystal_colour            'dark red'
_exptl_crystal_density_diffrn    1.870
_exptl_crystal_description       spline
_exptl_crystal_F_000             1452
_exptl_crystal_preparation       ', Luminescent'
_exptl_crystal_size_max          0.400
_exptl_crystal_size_mid          0.253
_exptl_crystal_size_min          0.160
_refine_diff_density_max         1.916
_refine_diff_density_min         -1.269
_refine_diff_density_rms         0.105
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     547
_refine_ls_number_reflns         11230
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.015
_refine_ls_R_factor_all          0.0379
_refine_ls_R_factor_gt           0.0281
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0476P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0727
_refine_ls_wR_factor_ref         0.0759
_reflns_Friedel_coverage         0.000
_reflns_number_gt                9191
_reflns_number_total             11230
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7cc01898c2.cif
_cod_data_source_block           P-1
_cod_database_code               7120034
_shelxl_version_number           2014-3
_shelx_res_checksum              46567